Tuning Morphology and Melting Temperature in spikelab/papers/148.pdfOptical microscopy images of a...
Embed Size (px)
Transcript of Tuning Morphology and Melting Temperature in spikelab/papers/148.pdfOptical microscopy images of a...
Tuning Morphology and Melting Temperature in Polyethylene Filmsby MAPLEHyuncheol Jeong, Mithun Chowdhury, Yucheng Wang, Melda Sezen-Edmonds, Yueh-Lin Loo,,
Richard A. Register,, Craig B. Arnold,, and Rodney D. Priestley*,,
Department of Chemical and Biological Engineering, Department of Mechanical and Aerospace Engineering, Princeton Institutefor the Science and Technology of Materials, and Andlinger Center for Energy and the Environment, Princeton University,Princeton, New Jersey 08544, United States
*S Supporting Information
ABSTRACT: The control of structure and thermal stability insemicrystalline polymer films remains an important challenge inapplications ranging from solar energy devices to packagingfilms. Here, we demonstrate the ability to dramatically alter themorphology and melting temperature (Tm) of low-molecular-weight linear polyethylene (PE) by employing an innovativevapor-assisted deposition process termed matrix assisted pulsedlaser evaporation (MAPLE). We report the ability to tune Tm ofPE films by 20 C by simply adjusting the depositiontemperature during MAPLE processing. This unique capabilitystems from the ability of MAPLE to exploit confinedcrystallization during thin film growth. In addition, wedemonstrate the ability to exploit MAPLE to design PE films that exhibit the same Tm as their melt-crystallized analoguesbut have an 25% higher degree of crystallinity. Our investigation offers new insights into how confinement effects in polymercrystallization can be utilized in the emerging field of polymer film fabrication by MAPLE to control structure and key materialproperties of semicrystalline polymer films.
INTRODUCTIONFrom next-generation solar energy harvesting devices1,2 tovarious types of plastic microelectronics,36 many of thepolymeric materials that will enable tomorrows technologiesare semicrystalline. Rather than comprising a single uniformphase, semicrystalline polymers are characterized by folded-chain lamellar crystals with intercalated entanglements thatremain amorphous.710 The structure within semicrystallinepolymers has a strong influence on thermal stability, i.e., themelting temperature (Tm) as well as the mechanical
1114 andelectrical10,1517 properties of semicrystalline polymers. Theprecise control of structure and Tm in polymer thin films,without the need for chemical modification13,1825 or theinclusion of functional additives,14,26 remains of interest and aformidable challenge in material science.Here, we introduce a new and promising approach to
dramatically tune the structure and Tm of semicrystallinepolymer films by exploiting the unique deposition capabilitiesof matrix assisted pulsed laser evaporation (MAPLE). In theMAPLE process, polymer films are grown by laser ablation of afrozen dilute solution of polymer and solvent, in which thesolvent serves as a sacrificial matrix to transport the polymerinto the gas phase and eliminate polymer degradation.27,28
MAPLE has been shown to be a promising approach to depositfunctional polymer films.2935 Via MAPLE, film growthproceeds by the deposition of nano- to micrometer-sized
isolated (or confined) polymer droplets with simultaneouscrystallization at a controlled substrate deposition temperature(Tdep).
36,37 By exploiting this feature, we demonstrate that forlow-molecular-weight linear polyethylene (PE; Mn = 3000, Mw/Mn = 1.10) Tm can be tuned by 20 C simply by controllingTdep during MAPLE deposition. To place these results incontext, it is not practically feasible to tune Tm by more than 5C via melt crystallization for PE.38,39 Furthermore, wedemonstrate that while PE films processed by MAPLE can bedesigned to exhibit the same Tm as their melt-crystallizedanalogues, the degree of crystallinity is always notablyenhanced. This tunability in the structure of PE stems fromthe ability of MAPLE to confine polymer crystallization intonanoscale dimensions during film formation.
RESULTS AND DISCUSSIONFilm Formation by Additive Deposition and Crystal-
lization of Confined PE Droplets. To gain an understandingof the crystallization mechanism of PE films formed by MAPLEprocessing, we first investigated the impact of Tdep oncrystallization during the early stages of film formation, i.e.,when the film consists of isolated nano- and microsized
Received: November 2, 2017Revised: December 14, 2017Published: January 10, 2018
Cite This: Macromolecules 2018, 51, 512519
2018 American Chemical Society 512 DOI: 10.1021/acs.macromol.7b02345Macromolecules 2018, 51, 512519
droplets of PE prior to consolidation. The importance of Tdepas a key processing parameter to control morphology, andhence properties, stems from its strong correlation to thenucleation rate of confined droplets and lamellar thickness.36
By characterizing the early stage film morphology, lamellarthicknesses and rough estimates of the critical volume (Vnucl)required for self-nucleation of the confined droplets could beinvestigated, as previously performed in the study of MAPLE-deposited poly(ethylene oxide).36,37 To enable such a study, wedeposited isolated PE droplets atop silicon substrates (Si) byMAPLE from a dilute solution target (see SupportingInformation for details of the MAPLE conditions).We first investigated the crystalline morphology formed at
Tdep = 116 C, which represents the typical crystallizationtemperature of bulk PE when Mn = 3000.
40 Figure 1a shows anoptical microscopy image of MAPLE-deposited PE (MAPLE-PE) droplets formed at Tdep = 116 C. At this temperature,platelet-like monolamellar crystals (MLCs) were formed fromnucleating confined droplets of volume larger than 1 m3.The region marked R1 in Figure 1a indicates a MLC grownfrom a nucleating droplet, whose structure is provided in theinset of Figure 1a. The AFM height image in Figure 1bmagnifies the MLC depicted in R1. This revealed that the MLChad a uniform thickness (lamellar thickness, d) of 27 nm,which agreed well with the fully extended chain length of PEwhen considering 0.127 nm as the increment of length per CH2group. It also agrees with the observation by Ueda andRegister,40 where the same PE, in bulk, formed extended chaincrystals when crystallized at a similar temperature. Theformation of 27 nm thick MLCs also indicated that themolecular weight of PE was well preserved during MAPLEprocessing.
When PE was deposited at Tdep = 75 C, the MLCs werecomposed of folded chains with d 10 nm. Interestingly,nucleating droplets with sizes down to 104103 m3 werecomposed of a single lamella or a few stacked lamellae, thusleading to the formation of PE nanocrystals. Figure 1c showsthe AFM amplitude image of the PE nanocrystals while Figure1d shows the AFM height image magnifying the region R2 inFigure 1c. The arrow in Figure 1c points to a crystal containinga screw dislocation, which represents the morphology of a fewstacked lamellae. The Figure 1c inset schematically describesthe structure of the PE nanocrystals. The nucleation rate forsuch small droplets (104103 m3) is expected to be highlydependent on Tc and the droplet size.
36,4143 The nucleationrate of PE confined to 103 m3 was predicted to be 1, 102,and 107 min1 at Tc = 75, 80, and 90 C, respectively.
Therefore, self-nucleation of such confined droplets wasexpected during the time scale of deposition (1 h) for Tdepbelow 80 C, but at Tdep above 80 C, only much largerdroplets would be able to nucleate during deposition. WhenTdep = 116 C, all identified nucleating droplets with d 27 nmhad a volume larger than 1 m3, as shown in Figure 1a.The above observations provided clues to PE film formation
and morphology development by MAPLE. In the early stages ofdeposition, crystallization of PE proceeds primarily vianucleation of droplets with volumes larger than Vnucl. As thefilm becomes consolidated, crystal lattice sites at the surface ofthe film promote the crystallization of subsequently depositeddroplets. Meanwhile, Tdep uniquely determines the thickness ofthe lamellae, as illustrated by Figure 1e, which compares therepresentative height profiles of MAPLE-PE MLCs formed atfour different Tdep: 75, 80, 100, and 116 C. The average MLCthickness at each Tdep is presented in Figure 1f. It should be
Figure 1. (a) Optical microscopy image of MAPLE-PE on Si formed with 30 min of deposition from a 0.2 mg/mL solution target at Tdep = 116 C.The inset shows the structure of a MLC grown from a nucleating droplet of size 1 m3. (b) AFM height image magnifying the MLC in R1 in parta. (c) AFM amplitude image of MAPLE-PE formed with Tdep = 75 C showing the morphology of PE nanocrystals consisting of a single lamella or afew stacked lamellae. The white arrow indicates a crystal with a screw dislocation. The inset schematic shows the structure of the PE nanocrystals.(d) AFM height image magnifying the MLCs in R2 in part c. (e) Representative height profiles of PE MLCs formed at various Tdep. (f) Bar graphcomparing MLC thicknesses of MAPLE-PE formed at various Tdep; error ranges represent the standard deviation of the height measurements onmultiple isolated PE MLCs formed at each Tdep.
Figure 2. (a) Optical microscopy image of MAPLE-PE on Si, formed with 1.5 h of deposition from a 1 mg/mL solution target at Tdep = 25 C. (b, c)Optical microscopy images of a flash-DSC chip where (b) shows the chip covered with a polyimide mask. The mask has a laser-machined hole of size250 250 m2 in the center (indicated by arrow), which exposes the sample stage of the chip. (c) Optical image that shows the sample stage of thechip after MAPLE PE deposition. The white dashed line marks the region of the deposited film.